Advanced Structured Materials Volume 17
Series Editors Andreas Öchsner Lucas F. M. da Silva Holm Altenbach
For furthe...

Author:
Mohd Nasir Tamin

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

Advanced Structured Materials Volume 17

Series Editors Andreas Öchsner Lucas F. M. da Silva Holm Altenbach

For further volumes: http://www.springer.com/series/8611

Mohd Nasir Tamin Editor

Damage and Fracture of Composite Materials and Structures

123

Mohd Nasir Tamin Faculty of Mechanical Engineering Universiti Teknologi Malaysia UTM Skudai 81310 Johor Malaysia e-mail: [email protected]

ISSN 1869-8433 ISBN 978-3-642-23658-7 DOI 10.1007/978-3-642-23659-4

e-ISSN 1869-8441 e-ISBN 978-3-642-23659-4

Springer Heidelberg Dordrecht London New York Library of Congress Control Number: 2011941716 Ó Springer-Verlag Berlin Heidelberg 2012 This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microfilm or in any other way, and storage in data banks. Duplication of this publication or parts thereof is permitted only under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer. Violations are liable to prosecution under the German Copyright Law. The use of general descriptive names, registered names, trademarks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Cover design: WMXDesign GmbH, Heidelberg Printed on acid-free paper Springer is part of Springer Science+Business Media (www.springer.com)

Preface

This book compiles recent advances in research and development in the area of damage and fracture of composite materials and structures. Majority of these chapters have been presented and discussed at the Special Session on Damage and Fracture of Composite Materials and Structures of the 4th International Conference on Advanced Computational Engineering and Experimenting (ACE-X), held during 8–10 July, 2010 in Paris, France. Invited chapters on selected topics are included. The scope of the book covers experimental, analytical and computational aspects of the mechanics of fibrous composites. The chapters report on updates related to testing of composite samples for determination of mechanical properties, discussion on the observed failure mechanisms and numerical modeling of deformation response of the composites to loading. Behavior of fibrous composites, sandwich structures and fiber-metal laminates to impact and blast loading are discussed. Response of composite structures under both static and dynamic loading is described. Each chapter is written as a self-contained report on recent research works of the respective authors. However, many issues related to damage and fracture of the composite are common. These include dominant fracture mechanisms, damagebased models and simulation approaches. The book is suitable not only for research, but also for advanced reference and applications. We acknowledge contributions from authors, many of whom are principal researchers of their projects on characterization of composite materials and structures. Thank you to Hassan Osman Ali for assistance in preparing this monograph. Johor, Malaysia, 2011

M. N. Tamin

v

Contents

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . M. N. Tamin

1

Mode-I Crack Control by SMA Fiber with a Special Configuration . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . M. Jin and S. H. Chen

5

Micromechanical Analysis of Mode I Crack Growth in Carbon Fibre Reinforced Polymers . . . . . . . . . . . . . . . . . . . . . . . . Daniel Trias and Pere Maimí

17

Modeling of Spalling Effect on Toughening in Fiber Reinforced Composites . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . C. Wang, N. F. Piaceski and K. M. Soares

27

Evolution Characteristics of Delamination Damage in CFRP Composites Under Transverse Loading . . . . . . . . . . . . . . . . S. S. R. Koloor, A. Abdul-Latif, X. J. Gong and M. N. Tamin

45

Indentation of Sandwich Beams with Functionally Graded Skins and Transversely Flexible Core . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Y. Mohammadi and S. M. R. Khalili

61

Micromechanical Fibre-Recruitment Model of Liquid Crystalline Polymer Reinforcing Polycarbonate Composites . . . . . . . . . . . . . . . . . K. L. Goh and L. P. Tan

85

vii

viii

Contents

Moisture Absorption Effects on the Resistance to Interlaminar Fracture of Woven Glass/Epoxy Composite Laminates . . . . . . . . . . . . X. J. Gong, K. J. Wong and M. N. Tamin

107

The Study of Response of High Performance Fiber-Reinforced Composites to Impact Loading. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . O. Saligheh, R. Eslami Farsani, R. Khajavi and M. Forouharshad

129

Dynamic Fracture Toughness of Composite Materials . . . . . . . . . . . . C. Rubio-González, J. Wang, J. Martinez and H. Kaur Impact Study on Aircraft Type Laminate Composite Plate; Experimental, Failure Criteria and Element Model Review . . . . . . . . Y. Aminanda The Blast Response of Sandwich Structures . . . . . . . . . . . . . . . . . . . . M. Yazid Yahya, W. J. Cantwell, G. S. Langdon and G. N. Nurick

143

157

189

The High Velocity Impact Response of Self-Reinforced Polypropylene Fibre Metal Laminates . . . . . . . . . . . . . . . . . . . . . . . . M. R. Abdullah and W. J. Cantwell

219

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

241

Introduction M. N. Tamin

Abstract Fiber-reinforced composites cover wide range of composite materials and structures including laminated panels of unidirectional plies, sandwich structures with fiber-reinforced composite skins and flexible core, and fiber-metal laminates. A typical advanced composite structure will likely experience quasistatic and dynamic loading. Under such damage-induced operating load conditions, reliability of the structure largely depends on the continual process of damage initiation and subsequent damage propagation to catastrophic fracture. The development of validated damage and failure models and availability of vast computing power would enable establishment of a validated framework for addressing structural reliability and safety issues of these composite structures. Keywords Fiber-reinforced composites Damage-based models damage mechanics Damage mechanisms Fatigue

Continuum

Fiber-reinforced composites cover wide range of composite materials and structures such as laminated panels of unidirectional plies, sandwich structures with fiber-reinforced composite skins and flexible core, and fiber-metal laminates (FML). Although glass and carbon fibers is relatively common, polymer, metal and ceramic fibers are being used as reinforcement phase in specific applications. Fiber-reinforced polymer (FRP) matrix composites offer an alternate replacement material to high-strength metals. In the transportation sector, the use of lightweight carbon fiber-reinforced polymer (CFRP) composites in airframe, automotive and railcar structures leads to improved (lower) fuel consumption and/or increased payload. The growth in use of CFRP composites from 15% in 1990

M. N. Tamin (&) Faculty of Mechanical Engineering, Center for Composites, Universiti Teknologi Malaysia (UTM), 81310 Skudai, Johor, Malaysia e-mail: [email protected]

M. N. Tamin (ed.), Damage and Fracture of Composite Materials and Structures, Advanced Structured Materials 17, DOI: 10.1007/978-3-642-23659-4_1, Ó Springer-Verlag Berlin Heidelberg 2012

1

2

M. N. Tamin

(A320) to over 50% in 2010 (A380) for airframe structures and high lift components is demonstrated [1]. The increasing use of CFRP composites is derived from its high strength-to-weight ratio, high specific modulus and flexible design through sequencing of the pre-impregnated laminates for tailored strength and stiffness properties in particular loading direction. The composite’s resistance to environmental corrosion is an added advantage over their metallic counterpart. This intrinsic property is appealing to applications in construction industry for bridges and wastewater and chemical storage tanks. Other property such as the composites transparency to radar is valuable for stealth applications. In numerous applications the composite structure will be subjected to both static and transient load throughout the design lives. As such, it is essential to identify dominant damage mechanisms and quantify failure process of the composite materials. This calls for evaluation of the materials resistance to quasi-static, impact and fatigue loading along with establishment of mechanical damage evolution. Reliability of the composite structure under such damage-induced operating load conditions depends on the continual process of damage initiation and subsequent damage propagation to catastrophic fracture. Such reliability data is indispensable during both initial material selection and detailed engineering design stage of a composite structure. Simple tests of the laminated composite coupons under tension, compression, shear and flexural loading are useful to measure intrinsic properties of the composites [2–4]. Fracture tests on pre-cracked samples are often used to establish fracture toughness and critical energy release rates of the composites in Mode I and II loadings [5]. However, specially-designed specimen, jigs and fixtures, and environmental chamber are required to establish mixed-mode loading effects [6], mean stress effects on fatigue life and moisture conditioning effects in accelerated testing [7]. The FRP composites ability to be fabricated into a wide range of laminated configurations can create costly materials evaluation programs. The magnitude of the test program could be reduced by implementing reliable life prediction models based on the properties and macro-lay-ups of the laminates. Failure process in FRP composites is a complex phenomenon. The different failure modes such as matrix yielding, matrix cracking, fiber/matrix interface de-bonding, fiber pull-out, fiber fracture and inter-ply delamination could occur in isolation or synergize simultaneously in FRP composites. An example of the various failure modes for unidirectional SiC fiber-reinforced titanium metal matrix composite is shown in Fig. 1. Additional fracture mechanisms observed following high-velocity impact and blast load are sheared, deformed and melted fibers, ductile tearing, thinning and sheared fracture of the metal in FMLs. Interface delamination in CFRP composites is of particular interest in view of the relatively weak ply-to-ply interface strength and the large interface shear stresses developed during loading. Interface delamination failure leads to significant loss of the loadcarrying capacity and occurs in the absence of any visible damage of the CFRP composite [8]. However, bridging crack growth observed in continuous fiberreinforced composites contributes to fracture toughness of the material through load shedding mechanisms [9]. Such critical delamination failure and bridging crack growth process could be accounted for in the design phase with the aid of

Introduction

3

Fig. 1 Bridging crack growth mechanism in SiC fiber-reinforced Ti-metal matrix composite illustrating fiber pull-out, fiber fracture, fiber/matrix interface debonding and matrix cracking. Fatigue crack growth test at 500 C, 10 Hz [9]

numerical modeling and validation testing of FRP composite specimens. In this respect, several materials models have been proposed and examined for predicting the composite strength with the different types of constituent defects. These include stress-based failure models [10–12] and strain-based criteria [13, 14] for matrix cracking and fiber fracture. Complete treatment of the mechanics of composite materials and the various failure models is best described in textbooks and handbooks [15–17]. The progression of each type of defects under fatigue load cycles dictates the useful life of the part. In this respect, cohesive zone model has been formulated for predicting ply interface delamination damage initiation and subsequent propagation under monotonic loading condition [18, 19]. The damagebased model employing virtual crack closure concept is introduced to account for load reversals in fatigue failure of the laminates [20, 21]. The simultaneous occurrence of multiple failure modes in a composite part under loading could not be represented by any of these models in isolation. To this end a unified approach based on continuum damage mechanics concept is much needed to account for the synergy effects of multiple failure mechanisms in FRP composites. Implementation of the newly-developed damage-based models into commercial finite element codes (e.g. [22]) and availability of vast computing power would yield a validated framework for addressing structural reliability and safety issues of FRP composite structures.

References 1. Baker, A.A., et al., (eds.).: Composite Materials for Aircraft Structures, 2nd edn. AIAA Education Series, USA (2004) 2. Standard Test Method for Tensile Properties of Polymer Matrix Composite Materials. ASTM Standard D3039/D3039 M-95a

4

M. N. Tamin

3. Standard Test Method for Compressive Properties of Unidirectional or Crossply Fiber-resin Composites. ASTM Standard D3410/3410 M-95 4. Standard Test Method for Shear Properties of Composite Materials by the V-Notched Beam Method. ASTM Standard D5379/D5379 M-93 5. Mode I Interlaminar Fracture Toughness of Unidirectional Fiber-Reinforced Polymer Matrix Composites, ASTM Standard D5528 (1994) 6. Benzeggagh, M.L., Kenane, M.: Measurement of Mixed-Mode Delamination Fracture Toughness of Unidirectional Glass/Epoxy Composites with Mixed-Mode Bending Apparatus. Compos. Sci. Technol. 49, 439–449 (1996) 7. Ciriscioli, P.R., Lee, W.I., Peterson, D.G.: Accelerated Environmental Testing of Composites. J. Compos. Mater. 21, 225–242 (1987) 8. Koloor, S.S.R., Abdul-Latif, A., Tamin, M.N.: Mechanics of Composite Delamination under Flexural Loading. Key Eng. Mater. 462–463, 726–731 (2011) 9. Tamin, M.N., Ghonem, H.: Fatigue Damage Mechanisms of Bridging Fibers in Titanium Metal Matrix Composites. J. Eng. Mater. Technol. Trans. ASME 122, 370–375 (2000) 10. Sun, C.T., Tao, J.X.: Prediction Failure Envelopes and Stress/Strain Behavior of Composite Laminates. Compos. Sci. Technol. 58, 1113–1125 (1998) 11. Hashin, Z., Rotem, A.: A Fatigue Failure Criterion for Fiber Reinforced Materials. J. Compos. Mater. 7, 448–464 (1973) 12. Tsai, S.W., Wu, E.M.: A General Theory of Strength for Anisotropic Materials. J. Compos. Mater. 5, 58–80 (1971) 13. Hart-Smith, L.J.: Prediction of the Original and Truncated Maximum Strain-Strain Failure Models for Certain Fibrous Composite Laminates. Compos. Sci. Technol. 58, 1151–1178 (1998) 14. Eckold, G.G.: Failure Criteria for Use in design Environment. Compos. Sci. Technol. 58, 1095–1105 (1998) 15. Chawla, K.K.: Composite Materials Science and Engineering. Springer, New York (1998) 16. Baker, A., Dutton, S., Kelly, D. (eds.).: Composite Materials for Aircraft Structures, 2nd edn. AIAA Inc., (2004) 17. Mallick, P.K. (ed.).: Composite Materials Handbook. Marcel Dekker, New York (1997) 18. Davila, C.G., Camanho, P.P., Moura, M.F.: Mixed-Mode Decohesion Elements for Analyses of Progressive Delamination. In: Proceedings of 42nd AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics and Materials Conference, Seattle, WA, 16–19 April (2001) 19. Turon, A., Camanho, P.P., Costa, J., Davila, C.G.: An Interface Damage Model for the Simulation of Delamination Under Variable-Mode Ratio in Composite Materials. NASA/ TM-2004–213277. VA, USA (2004) 20. Krueger, R.: The Virtual Crack Closure Technique: History, Approach and Application. NASA/CR-2002–211628. NTIS, VA, USA (2002) 21. Xie, D., Biggers Jr., S.B.: Progressive Crack growth Analysis using Interface Element based on Virtual Crack Closure Technique. Finite Elem. Anal. Desi. 42, 977–984 (2006) 22. Abaqus ver 6.9, Simulia Inc.

Mode-I Crack Control by SMA Fiber with a Special Configuration M. Jin and S. H. Chen

Abstract Crack propagation in solid members is an important reason for structure failure. In recent years, many research interests are focused on intelligent control of crack propagation. With the rise in temperature, contraction of prestrained SMA fiber embedded in matrix makes retardation of crack propagation possible. However, with the rise in temperature, separation of SMA fiber from matrix is inevitable. This kind of separation weakens effect of SMA fiber on crack tip. To overcome de-bonding of SMA fiber from matrix, a knot is made on the fiber in this paper. By shape memory effect with the rise in temperature, the knotted SMA fiber generates a couple of recovery forces acting on the matrix at the two knots. This couple of recovery forces may restrain opening of the mode-I crack. Based on Tanaka constitutive law on SMA fiber and complex stress function near an elliptic hole under a point load, a theoretical model on mode-I crack is proposed. An analytical expression of relation between stress intensity factor (SIF) of mode-I crack closure and temperature is got. Simulation results show that stress intensity factor of mode-I crack closure decreases obviously with the rise in temperature higher than the austenite start temperature of SMA fiber, and that there is an optimal position for SMA fiber to restrain crack opening, which is behind the crack tip. Therefore the theoretical model supports that prestrained SMA fiber with knots in martensite can be used to control mode-I crack opening effectively because de-bonding between fiber and matrix is eliminated. Specimen of epoxy resin embedded with knotted SMA fiber can be made in experiment and is useful to an

M. Jin (&) S. H. Chen The State Key Laboratory of Nonlinear Mechanics (LNM), Beijing 100190, People’ s Republic of China e-mail: [email protected] M. Jin Department of Mechanics, School of Civil Engineering, Beijing Jiaotong University, Beijing 100044, People’ s Republic of China

M. N. Tamin (ed.), Damage and Fracture of Composite Materials and Structures, Advanced Structured Materials 17, DOI: 10.1007/978-3-642-23659-4_2, Ó Springer-Verlag Berlin Heidelberg 2012

5

6

M. Jin and S. H. Chen

analytical study. However, in practical point of view, SMA fiber should be embedded in engineering structure material such as steel, aluminum, etc. The embedding process in these matrix materials should be studied systematically in the future. Keywords Crack control

SMA fiber Actuator Complex stress function

1 Introduction Crack propagation in solid members is an important reason for structure failure. Many researchers are interested in methods of crack control. With the rise in temperature, contraction of prestrained shape memory alloy (SMA) fiber embedding in matrix makes retardation of crack propagation possible. Rogers et al. [1] proposed that embedded prestrained SMA fiber near crack tip may reduce the stress by contraction effect of SMA under increase of temperature. Photoelastic pictures and finite element analysis show that stress intensity factor (SIF) of a specimen embedded with prestrained SMA fiber decreased as temperature increases [2–4]. To overcome separation of SMA fiber from matrix, surface of SMA fiber is treated chemically [2]. Shimamoto et al. [5–8] and Umezaki et al. [9] indicated that stress at the tip of mode-I crack in epoxy matrix with SMA fiber can be reduced by heating SMA fiber. Quality change in matrix near SMA fiber is observed if the temperature is too high. This kind of quality change damages the contraction effect of SMA fiber on crack closure in matrix. Araki et al. [10, 11] performed a micromechanical model on crack closure considering crack bridging fibers and compared their numerical results with experiment. Experiments in these researches give a possible way in practical use to control crack propagation in a specimen. However, with the rise in temperature, separation of SMA fiber from matrix is inevitable. This kind of separation weakens effect of SMA fiber on crack tip. In other words, effect of those applications is limited by the interfacial debonding. Umezaki [12] proposed a type of spiral SMA wire to prevent separation of SMA wire from matrix. In order to avoid the interface de-cohesion or sliding, Gabry et al. [13] used different surface treatments on SMA wires. Pullout tests and scanning electronic microscopy observations [14] indicated that increasing the number of turns of the twisted NiTi wires strengthens bonding strength between fiber and matrix. Zhou et al. [15–17] studied SMA fiber debonding in matrix. Wang et al. [18] proposed a theoretical model for SMA pullout from an elastic matrix. Hu et al. [19] studied interface failure between SMA fiber and matrix by shear lag model. Considering debonding at the interface between SMA wires and a polymer matrix, Wang [20] estimated the minimum volume fraction of SMA wires required to produce stress for the active crack closure. By finite element simulation, Burton et al. [21] indicated that reverse transformation of SMA wires during heating causes a closure force across the crack.

Mode-I Crack Control by SMA Fiber

7

knotted SMA fiber

h crack

a

a

l s

h

photo of a knot

Fig. 1 A knotted prestrained SMA fiber perpendicular to crack surface

To improve effect of SMA fiber on matrix, small knots on SMA fiber are made by authors. Figure 1 shows configuration of a prestrained SMA fiber with knots at each end. With the rise in temperature, the SMA fiber contracts and the two knots on the fiber locking tightly on matrix by recovery stress. This recovery force may reduce the stress intensity factor at the crack tip and make the crack closure. In this process, the fiber cannot be debonded from matrix totally. Therefore, as an actuator in practical use, knotted SMA fiber can be embedded in matrix to control crack propagation. Relation of stress intensity factor with temperature is an important problem in crack control. In this paper, an approximate model on stress intensity factor of mode-I crack closure in matrix is proposed on a specimen with embedded SMA fiber with knots.

2 Relation of Recovery Force on Matrix with Temperature See Fig. 1. Considering a specimen with a mode-I crack in matrix embedded with a prestrained SMA fiber with knots in martensite. SMA fiber is perpendicular to crack surface. Plane strain problem is considered. 2a and 2h denote length of crack and length between the two knots, respectively. l denotes distance from the right crack tip to the fiber. With the rise in temperature, the knotted SMA fiber contracts due to phase transformation from martensite to austenite. The SMA fiber generates a couple of recovery forces P at upper knot Z0 and P at lower knot Z 0 acting on matrix where Z0 ¼ a þ l þ ih;

ð1Þ

8

M. Jin and S. H. Chen

Fig. 2 A couple of recovery forces, P acting on matrix

P y Z0 h x l

h

Z

0

P

Z 0 denotes conjugate of Z0 ; and i denotes imaginary unit. See Fig. 2. Because bonding on interface between fiber and matrix is much weaker than locking between knot and matrix, interfacial shear stress is neglected in this paper. Therefore, the knotted SMA fiber is in simple tension by axial load, P. We have P ¼ srf ;

ð2Þ

where rf and s denote recovery stress and area of the SMA fiber, respectively. In phase transformation, strain of SMA fiber is about several percent which is one order higher than strain of epoxy in elastic range. So we neglect strain of matrix when we consider strain of SMA fiber. Because each knot is locked in the matrix as the fiber contracts, increase of normal strain of SMA fiber embedding in the matrix is approximately zero, i.e. def ¼ 0;

ð3Þ

where ef denotes normal strain of SMA fiber in phase transformation. Based on the Tanaka one-dimensional constitutive law on SMA [22], we have drf ¼ Ef def þ H dT þ X dn;

ð4Þ

where Ef denotes Young’s modulus; H denotes thermoelastic modulus; and X denotes phase transformation modulus. If eL denotes maximum residual strain, we have X ¼ Ef eL in SMA fiber. drf , dT and dn denote increase of normal stress, rise in temperature and increase of martensitic volume fraction of SMA fiber. Martensitic volume fraction, n is a function of stress, rf and temperature, T , i.e., n ¼ n rf ; T : ð5Þ Substituting Eqs. 3 to 5 into 4, we have increase of recovery stress

Mode-I Crack Control by SMA Fiber Fig. 3 Recovery stress, rf versus temperature, T

f

9

£¨ MPa£©

600

400

200

0 40

50

60

70

o

T(C)

drf ¼

on H þ X oT on 1 X or f

dT :

ð6Þ

In phase transformation from martensite to austenite with rise in temperature, function (5) can be approximated by an exponential function [22] with respect to temperature, T , i.e., ð7Þ n ¼ exp aA ðAs T Þ þ bA rf ; aA ln 10 where aA ¼ 2 As Af ; bA ¼ CA ; As and Af are austenite start temperature and austenite finish temperature of SMA fiber, respectively; CA denotes influence coefficient of stress on transition temperature. Substituting Eq. 7 into 6, we have H aA X exp aA ðAs T Þ þ bA rf dT : drf ¼ ð8Þ 1 bA X exp aA ðAs T Þ þ bA rf

Before heating the SMA fiber, stress in theSMA fiber is zero as temperature, T As . The initial value of rf in Eq. 8 is rf T¼As ¼ 0. Generally, we can solve initial value problem (8) numerically by the Euler iteration. However, in Appendix A, we have an analytical solution of initial value problem (8) on martensitic volume fraction, n 8 ln n bA Xðn 1Þ > > þ As ln n aA ðAs T Þ > : rf ¼ bA where n decreases at 1. For a given n, we can get T and rf from Eq. 9. Substituting the value of rf into Eq. 2, we have relation of point load, P with temperature, T : Figure 3 shows curve of recovery stress, rf versus temperature, T .

10

M. Jin and S. H. Chen

Table 1 Material Properties of NiTi Fiber [16, 21] eL As Af Ef 37.4 GPa

0.067

37.7oC

47.2oC

H

CA

9.1 MPa/oC

20.3 MPa/oC

3 Stress Intensity Factor of Mode-I Crack Closure Under a Couple of Point Loads Complex stress function of an elliptic hole in plane strain under a point load is given by [23]. The elliptic hole degenerates into a crack in Fig. 1 as perpendicular axis of elliptic hole tends to zero. Thus we can get complex stress function of the crack under a point load. Based on this complex stress function, we can get stress intensity factor of mode-I crack closure under a couple of point loads P in Fig. 2. The formulation can be seen in Appendix B. Considering Eq. 2, we have ( #) " pﬃﬃﬃ 2 rf 1 1 f a 0 þ ð1 þ m0 ÞIm f0 þ Re ; KI ¼ pﬃﬃﬃ 2Im f0 1 f0 s p ðf0 þ 1Þðf0 1Þ3 ð10Þ where KI is the stress intensity factor of mode-I crack closure, f0 is given by a 1 m where m denotes Poisson’s ratio of matrix; ReðÞ and ImðÞ Z0 ¼ 2 f0 þ f0 ; m0 ¼ 1m denote real component and imaginary component of ðÞ, respectively. Recovery stress, rf can be calculated numerically from Eq. 8 under a temperature, T or analytically from Eq. 9. Substituting recovery stress, rf into Eq. 10, we have the stress intensity factor, KI of mode-I crack closure. Then we have relation of the stress intensity factor, KI of mode-I crack closure with temperature, T .

4 Numerical Results Material properties of SMA fiber are listed in Table l, where Ef denotes Young’s modulus; eL denotes maximum residual strain; As denotes austenite start temperature; Af denotes austenite finish temperature; H denotes thermoelastic modulus; CA denotes influence coefficient of stress on transition temperature. Poisson’s ratio of matrix is m ¼ 0:3. Figure 3 shows curve of recovery stress, rf versus temperature, T . It is shown that recovery stress, rf reaches about 600 MPa as temperature rises to 70 C. Figure 4 shows martensitic volume fraction, n as a function with respect to temperature, T in phase transformation in Figs. 5, 6, 7, 8 and 9. It is shown that martensitic volume fraction, n decreases as the temperature rises from 40 to 70 C:

Mode-I Crack Control by SMA Fiber Fig. 4 Martensitic volume fraction, ξ versus temperature, T

11

1.00

0.95

0.90

0.85

40

50

60

o

70

T ( C)

Fig. 5 The closure stress intensity factor, KI versus temperature, T for different fiber position as h/a = 1.0

a

1/2

K I /s ( Pa ) l/a = -1.0

0

-0.8 -100

-0.6

-200

-0.4

-300 -400 -500 40

50

60

70

T ( oC )

a

1/2

K I /s ( Pa )

l / a = 0.8

0.6 0.4

0

0.2 -100 -200 0.0

-300

-0.2

-400 -500 40

50

T ( oC )

60

70

12 Fig. 6 The closure stress intensity factor, KI versus fiber position, l/a at different temperature as h/a = 1.0

M. Jin and S. H. Chen a

1/2

K I /s ( Pa ) o

0

T = 40 C 45

-100

50 55

-200

60 65

-300

70 -400 -500

l/a -1.5

Fig. 7 The closure stress intensity factor, KI versus fiber position, l/a at different temperature as h/a = 0.1

-1.0

-0.5

0.0

0.5

1.0

1/2

a K I /s ( Pa ) T = 40o C 0 45 -500

50 55

-1000

60 65

-1500 70

l/a -2000 -1.5

Fig. 8 The closure stress intensity factor, KI versus fiber position l/a at different temperature as h/a = 2.0

-1.0

-0.5

0.0

0.5

1.0

-0.5

0.0

0.5

1.0

1/2

a K I /s ( Pa ) 0

T = 40 oC 45

-100

50 55 60

-200

65 70

-300 -1.5

l/a -1.0

As crack length is the same as fiber length, i.e. ha ¼ 1:0, Fig. 5 shows the stress intensity factor of mode-I crack closure as function with respect to temperature for different fiber position. It is shown that stress intensity factor decreases almost

Mode-I Crack Control by SMA Fiber Fig. 9 The closure stress intensity factor, KI versus fiber position l/a at different fiber length

13

1/2

a K I /s ( Pa )

T = 40 oC

0

-40 1.5 1.0

-80

0.5 h /a = 0.1

-120

l/a -1.0

-0.5

0.0

0.5

1.0

linearly with rise in temperature. It is shown that stress intensity factor may take the minimum value at the same temperature between al ¼ 0:2 and 0:4. Figure 6 shows closure stress intensity factor as a function with respect to fiber position at different temperature. At the same temperature, the nearer the fiber locates the crack tip, the little the stress intensity factor is. Effect of crack closure of the fiber behind crack tip is more obvious than that of the fiber in front of crack tip. It is also shown that there is an optimal position for fiber where the stress intensity factor takes the minimum value. For ha ¼ 1:0, this optimal position for effect of crack closure is approximately at al ¼ 0:3 behind the crack tip. Figures 7 and 8 show the stress intensity factor of mode-I crack closure as a function with respect to fiber position at different temperature for ha ¼ 0:1 and 2:0, respectively. Approximately l a ¼ 0:04 and 0:45 are the optimal position for effect of crack closure for h a ¼ 0:1 and 2:0, respectively. Figure 9 shows the closure stress intensity factor as a function with respect to fiber position al for different fiber length ha at temperature 40 C. Near the crack tip, it is shown that, the more short distance of the two knots is, the more obvious the effect of crack closure is. In other words, the nearer the knot locates the crack tip, the more obvious effect of crack closure is.

5 Conclusions Based on the Tanaka one-dimensional constitutive law on SMA, an approximate model on stress intensity factor of mode-I crack closure by prestrained knotted SMA fiber in martensite is proposed. Relation of the stress intensity factor of mode-I crack closure with temperature is given in Eqs. 8 and 9. Numerical results show that the stress intensity factor of mode-I crack closure increases as the prestrained knotted SMA fiber in martensite is heated. Optimal position of the knotted SMA fiber for crack closure is behind the crack tip. As an actuator in

14

M. Jin and S. H. Chen

matrix, prestrained knotted SMA fiber in martensite can be used to control mode-I crack opening. Acknowledgments Authors gratefully acknowledge support from Opening Fund of State Key Laboratory of Nonlinear Mechanics (LNM) of Chinese Academy of Sciences, P. R. China, through grant number LNM201003 and the Science Foundation of Beijing Jiaotong University through grant number PD-225.

Appendix A From derivative of Eq. 7 with respect to temperature, T , we have drf 1 dn ¼ þ aA : dT bA ndT

ðA1Þ

Substituting Eqs. 7 and (A1) into 8, we have 1 bA X dn ¼ ðbA H aA ÞdT : n

ðA2Þ

Indefinite integral of Eq. A2 is ln n bA Xn þ c: ðA3Þ b A H aA where c is a constant. Substituting rf T ¼As ¼ 0 into Eqs. 7 and A3, we have T¼

c¼

bA X þ As : b A H aA

ðA4Þ

Substituting Eq. A4 into A3, we have the first equation in Eq. 9. The second equation in Eq. 9 can be got easily from Eq. 7.

Appendix B Complex stress functions UðfÞ and vðfÞ of an elliptic hole in plane strain under a point load P at Z0 in Fig. 2. are given in Eqs. 4 and 5 in article of [23], respectively. As perpendicular axis of the elliptic hole tends to zero, we have derivatives of UðfÞ and vðfÞ with respect to f 8 2

39 ! > > 1 1 = 2< f þ þ f 0 0 f0 7 dUðfÞ iPa 1 1 f0 0 0 6 1 ¼ þ 1 þ m ð3 m Þ ð Þ þ 5 4

2 2 > 8p > df f f0 f 1 f ; : f0 f0 1 f 1 f0

ðB1Þ

Mode-I Crack Control by SMA Fiber

15

and

39 1 1 = f f þ þ 0 0 f0 dvðfÞ iPa 3m 1 1 f0 5 ; ðB2Þ

þ ð1 þ m0 Þ4 ¼ þ ; 8p :f f0 df f 1 f ðf f0 Þ2 1 f12 f0 8

2

Series Editors Andreas Öchsner Lucas F. M. da Silva Holm Altenbach

For further volumes: http://www.springer.com/series/8611

Mohd Nasir Tamin Editor

Damage and Fracture of Composite Materials and Structures

123

Mohd Nasir Tamin Faculty of Mechanical Engineering Universiti Teknologi Malaysia UTM Skudai 81310 Johor Malaysia e-mail: [email protected]

ISSN 1869-8433 ISBN 978-3-642-23658-7 DOI 10.1007/978-3-642-23659-4

e-ISSN 1869-8441 e-ISBN 978-3-642-23659-4

Springer Heidelberg Dordrecht London New York Library of Congress Control Number: 2011941716 Ó Springer-Verlag Berlin Heidelberg 2012 This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specifically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microfilm or in any other way, and storage in data banks. Duplication of this publication or parts thereof is permitted only under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer. Violations are liable to prosecution under the German Copyright Law. The use of general descriptive names, registered names, trademarks, etc. in this publication does not imply, even in the absence of a specific statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Cover design: WMXDesign GmbH, Heidelberg Printed on acid-free paper Springer is part of Springer Science+Business Media (www.springer.com)

Preface

This book compiles recent advances in research and development in the area of damage and fracture of composite materials and structures. Majority of these chapters have been presented and discussed at the Special Session on Damage and Fracture of Composite Materials and Structures of the 4th International Conference on Advanced Computational Engineering and Experimenting (ACE-X), held during 8–10 July, 2010 in Paris, France. Invited chapters on selected topics are included. The scope of the book covers experimental, analytical and computational aspects of the mechanics of fibrous composites. The chapters report on updates related to testing of composite samples for determination of mechanical properties, discussion on the observed failure mechanisms and numerical modeling of deformation response of the composites to loading. Behavior of fibrous composites, sandwich structures and fiber-metal laminates to impact and blast loading are discussed. Response of composite structures under both static and dynamic loading is described. Each chapter is written as a self-contained report on recent research works of the respective authors. However, many issues related to damage and fracture of the composite are common. These include dominant fracture mechanisms, damagebased models and simulation approaches. The book is suitable not only for research, but also for advanced reference and applications. We acknowledge contributions from authors, many of whom are principal researchers of their projects on characterization of composite materials and structures. Thank you to Hassan Osman Ali for assistance in preparing this monograph. Johor, Malaysia, 2011

M. N. Tamin

v

Contents

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . M. N. Tamin

1

Mode-I Crack Control by SMA Fiber with a Special Configuration . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . M. Jin and S. H. Chen

5

Micromechanical Analysis of Mode I Crack Growth in Carbon Fibre Reinforced Polymers . . . . . . . . . . . . . . . . . . . . . . . . Daniel Trias and Pere Maimí

17

Modeling of Spalling Effect on Toughening in Fiber Reinforced Composites . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . C. Wang, N. F. Piaceski and K. M. Soares

27

Evolution Characteristics of Delamination Damage in CFRP Composites Under Transverse Loading . . . . . . . . . . . . . . . . S. S. R. Koloor, A. Abdul-Latif, X. J. Gong and M. N. Tamin

45

Indentation of Sandwich Beams with Functionally Graded Skins and Transversely Flexible Core . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Y. Mohammadi and S. M. R. Khalili

61

Micromechanical Fibre-Recruitment Model of Liquid Crystalline Polymer Reinforcing Polycarbonate Composites . . . . . . . . . . . . . . . . . K. L. Goh and L. P. Tan

85

vii

viii

Contents

Moisture Absorption Effects on the Resistance to Interlaminar Fracture of Woven Glass/Epoxy Composite Laminates . . . . . . . . . . . . X. J. Gong, K. J. Wong and M. N. Tamin

107

The Study of Response of High Performance Fiber-Reinforced Composites to Impact Loading. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . O. Saligheh, R. Eslami Farsani, R. Khajavi and M. Forouharshad

129

Dynamic Fracture Toughness of Composite Materials . . . . . . . . . . . . C. Rubio-González, J. Wang, J. Martinez and H. Kaur Impact Study on Aircraft Type Laminate Composite Plate; Experimental, Failure Criteria and Element Model Review . . . . . . . . Y. Aminanda The Blast Response of Sandwich Structures . . . . . . . . . . . . . . . . . . . . M. Yazid Yahya, W. J. Cantwell, G. S. Langdon and G. N. Nurick

143

157

189

The High Velocity Impact Response of Self-Reinforced Polypropylene Fibre Metal Laminates . . . . . . . . . . . . . . . . . . . . . . . . M. R. Abdullah and W. J. Cantwell

219

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

241

Introduction M. N. Tamin

Abstract Fiber-reinforced composites cover wide range of composite materials and structures including laminated panels of unidirectional plies, sandwich structures with fiber-reinforced composite skins and flexible core, and fiber-metal laminates. A typical advanced composite structure will likely experience quasistatic and dynamic loading. Under such damage-induced operating load conditions, reliability of the structure largely depends on the continual process of damage initiation and subsequent damage propagation to catastrophic fracture. The development of validated damage and failure models and availability of vast computing power would enable establishment of a validated framework for addressing structural reliability and safety issues of these composite structures. Keywords Fiber-reinforced composites Damage-based models damage mechanics Damage mechanisms Fatigue

Continuum

Fiber-reinforced composites cover wide range of composite materials and structures such as laminated panels of unidirectional plies, sandwich structures with fiber-reinforced composite skins and flexible core, and fiber-metal laminates (FML). Although glass and carbon fibers is relatively common, polymer, metal and ceramic fibers are being used as reinforcement phase in specific applications. Fiber-reinforced polymer (FRP) matrix composites offer an alternate replacement material to high-strength metals. In the transportation sector, the use of lightweight carbon fiber-reinforced polymer (CFRP) composites in airframe, automotive and railcar structures leads to improved (lower) fuel consumption and/or increased payload. The growth in use of CFRP composites from 15% in 1990

M. N. Tamin (&) Faculty of Mechanical Engineering, Center for Composites, Universiti Teknologi Malaysia (UTM), 81310 Skudai, Johor, Malaysia e-mail: [email protected]

M. N. Tamin (ed.), Damage and Fracture of Composite Materials and Structures, Advanced Structured Materials 17, DOI: 10.1007/978-3-642-23659-4_1, Ó Springer-Verlag Berlin Heidelberg 2012

1

2

M. N. Tamin

(A320) to over 50% in 2010 (A380) for airframe structures and high lift components is demonstrated [1]. The increasing use of CFRP composites is derived from its high strength-to-weight ratio, high specific modulus and flexible design through sequencing of the pre-impregnated laminates for tailored strength and stiffness properties in particular loading direction. The composite’s resistance to environmental corrosion is an added advantage over their metallic counterpart. This intrinsic property is appealing to applications in construction industry for bridges and wastewater and chemical storage tanks. Other property such as the composites transparency to radar is valuable for stealth applications. In numerous applications the composite structure will be subjected to both static and transient load throughout the design lives. As such, it is essential to identify dominant damage mechanisms and quantify failure process of the composite materials. This calls for evaluation of the materials resistance to quasi-static, impact and fatigue loading along with establishment of mechanical damage evolution. Reliability of the composite structure under such damage-induced operating load conditions depends on the continual process of damage initiation and subsequent damage propagation to catastrophic fracture. Such reliability data is indispensable during both initial material selection and detailed engineering design stage of a composite structure. Simple tests of the laminated composite coupons under tension, compression, shear and flexural loading are useful to measure intrinsic properties of the composites [2–4]. Fracture tests on pre-cracked samples are often used to establish fracture toughness and critical energy release rates of the composites in Mode I and II loadings [5]. However, specially-designed specimen, jigs and fixtures, and environmental chamber are required to establish mixed-mode loading effects [6], mean stress effects on fatigue life and moisture conditioning effects in accelerated testing [7]. The FRP composites ability to be fabricated into a wide range of laminated configurations can create costly materials evaluation programs. The magnitude of the test program could be reduced by implementing reliable life prediction models based on the properties and macro-lay-ups of the laminates. Failure process in FRP composites is a complex phenomenon. The different failure modes such as matrix yielding, matrix cracking, fiber/matrix interface de-bonding, fiber pull-out, fiber fracture and inter-ply delamination could occur in isolation or synergize simultaneously in FRP composites. An example of the various failure modes for unidirectional SiC fiber-reinforced titanium metal matrix composite is shown in Fig. 1. Additional fracture mechanisms observed following high-velocity impact and blast load are sheared, deformed and melted fibers, ductile tearing, thinning and sheared fracture of the metal in FMLs. Interface delamination in CFRP composites is of particular interest in view of the relatively weak ply-to-ply interface strength and the large interface shear stresses developed during loading. Interface delamination failure leads to significant loss of the loadcarrying capacity and occurs in the absence of any visible damage of the CFRP composite [8]. However, bridging crack growth observed in continuous fiberreinforced composites contributes to fracture toughness of the material through load shedding mechanisms [9]. Such critical delamination failure and bridging crack growth process could be accounted for in the design phase with the aid of

Introduction

3

Fig. 1 Bridging crack growth mechanism in SiC fiber-reinforced Ti-metal matrix composite illustrating fiber pull-out, fiber fracture, fiber/matrix interface debonding and matrix cracking. Fatigue crack growth test at 500 C, 10 Hz [9]

numerical modeling and validation testing of FRP composite specimens. In this respect, several materials models have been proposed and examined for predicting the composite strength with the different types of constituent defects. These include stress-based failure models [10–12] and strain-based criteria [13, 14] for matrix cracking and fiber fracture. Complete treatment of the mechanics of composite materials and the various failure models is best described in textbooks and handbooks [15–17]. The progression of each type of defects under fatigue load cycles dictates the useful life of the part. In this respect, cohesive zone model has been formulated for predicting ply interface delamination damage initiation and subsequent propagation under monotonic loading condition [18, 19]. The damagebased model employing virtual crack closure concept is introduced to account for load reversals in fatigue failure of the laminates [20, 21]. The simultaneous occurrence of multiple failure modes in a composite part under loading could not be represented by any of these models in isolation. To this end a unified approach based on continuum damage mechanics concept is much needed to account for the synergy effects of multiple failure mechanisms in FRP composites. Implementation of the newly-developed damage-based models into commercial finite element codes (e.g. [22]) and availability of vast computing power would yield a validated framework for addressing structural reliability and safety issues of FRP composite structures.

References 1. Baker, A.A., et al., (eds.).: Composite Materials for Aircraft Structures, 2nd edn. AIAA Education Series, USA (2004) 2. Standard Test Method for Tensile Properties of Polymer Matrix Composite Materials. ASTM Standard D3039/D3039 M-95a

4

M. N. Tamin

3. Standard Test Method for Compressive Properties of Unidirectional or Crossply Fiber-resin Composites. ASTM Standard D3410/3410 M-95 4. Standard Test Method for Shear Properties of Composite Materials by the V-Notched Beam Method. ASTM Standard D5379/D5379 M-93 5. Mode I Interlaminar Fracture Toughness of Unidirectional Fiber-Reinforced Polymer Matrix Composites, ASTM Standard D5528 (1994) 6. Benzeggagh, M.L., Kenane, M.: Measurement of Mixed-Mode Delamination Fracture Toughness of Unidirectional Glass/Epoxy Composites with Mixed-Mode Bending Apparatus. Compos. Sci. Technol. 49, 439–449 (1996) 7. Ciriscioli, P.R., Lee, W.I., Peterson, D.G.: Accelerated Environmental Testing of Composites. J. Compos. Mater. 21, 225–242 (1987) 8. Koloor, S.S.R., Abdul-Latif, A., Tamin, M.N.: Mechanics of Composite Delamination under Flexural Loading. Key Eng. Mater. 462–463, 726–731 (2011) 9. Tamin, M.N., Ghonem, H.: Fatigue Damage Mechanisms of Bridging Fibers in Titanium Metal Matrix Composites. J. Eng. Mater. Technol. Trans. ASME 122, 370–375 (2000) 10. Sun, C.T., Tao, J.X.: Prediction Failure Envelopes and Stress/Strain Behavior of Composite Laminates. Compos. Sci. Technol. 58, 1113–1125 (1998) 11. Hashin, Z., Rotem, A.: A Fatigue Failure Criterion for Fiber Reinforced Materials. J. Compos. Mater. 7, 448–464 (1973) 12. Tsai, S.W., Wu, E.M.: A General Theory of Strength for Anisotropic Materials. J. Compos. Mater. 5, 58–80 (1971) 13. Hart-Smith, L.J.: Prediction of the Original and Truncated Maximum Strain-Strain Failure Models for Certain Fibrous Composite Laminates. Compos. Sci. Technol. 58, 1151–1178 (1998) 14. Eckold, G.G.: Failure Criteria for Use in design Environment. Compos. Sci. Technol. 58, 1095–1105 (1998) 15. Chawla, K.K.: Composite Materials Science and Engineering. Springer, New York (1998) 16. Baker, A., Dutton, S., Kelly, D. (eds.).: Composite Materials for Aircraft Structures, 2nd edn. AIAA Inc., (2004) 17. Mallick, P.K. (ed.).: Composite Materials Handbook. Marcel Dekker, New York (1997) 18. Davila, C.G., Camanho, P.P., Moura, M.F.: Mixed-Mode Decohesion Elements for Analyses of Progressive Delamination. In: Proceedings of 42nd AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics and Materials Conference, Seattle, WA, 16–19 April (2001) 19. Turon, A., Camanho, P.P., Costa, J., Davila, C.G.: An Interface Damage Model for the Simulation of Delamination Under Variable-Mode Ratio in Composite Materials. NASA/ TM-2004–213277. VA, USA (2004) 20. Krueger, R.: The Virtual Crack Closure Technique: History, Approach and Application. NASA/CR-2002–211628. NTIS, VA, USA (2002) 21. Xie, D., Biggers Jr., S.B.: Progressive Crack growth Analysis using Interface Element based on Virtual Crack Closure Technique. Finite Elem. Anal. Desi. 42, 977–984 (2006) 22. Abaqus ver 6.9, Simulia Inc.

Mode-I Crack Control by SMA Fiber with a Special Configuration M. Jin and S. H. Chen

Abstract Crack propagation in solid members is an important reason for structure failure. In recent years, many research interests are focused on intelligent control of crack propagation. With the rise in temperature, contraction of prestrained SMA fiber embedded in matrix makes retardation of crack propagation possible. However, with the rise in temperature, separation of SMA fiber from matrix is inevitable. This kind of separation weakens effect of SMA fiber on crack tip. To overcome de-bonding of SMA fiber from matrix, a knot is made on the fiber in this paper. By shape memory effect with the rise in temperature, the knotted SMA fiber generates a couple of recovery forces acting on the matrix at the two knots. This couple of recovery forces may restrain opening of the mode-I crack. Based on Tanaka constitutive law on SMA fiber and complex stress function near an elliptic hole under a point load, a theoretical model on mode-I crack is proposed. An analytical expression of relation between stress intensity factor (SIF) of mode-I crack closure and temperature is got. Simulation results show that stress intensity factor of mode-I crack closure decreases obviously with the rise in temperature higher than the austenite start temperature of SMA fiber, and that there is an optimal position for SMA fiber to restrain crack opening, which is behind the crack tip. Therefore the theoretical model supports that prestrained SMA fiber with knots in martensite can be used to control mode-I crack opening effectively because de-bonding between fiber and matrix is eliminated. Specimen of epoxy resin embedded with knotted SMA fiber can be made in experiment and is useful to an

M. Jin (&) S. H. Chen The State Key Laboratory of Nonlinear Mechanics (LNM), Beijing 100190, People’ s Republic of China e-mail: [email protected] M. Jin Department of Mechanics, School of Civil Engineering, Beijing Jiaotong University, Beijing 100044, People’ s Republic of China

M. N. Tamin (ed.), Damage and Fracture of Composite Materials and Structures, Advanced Structured Materials 17, DOI: 10.1007/978-3-642-23659-4_2, Ó Springer-Verlag Berlin Heidelberg 2012

5

6

M. Jin and S. H. Chen

analytical study. However, in practical point of view, SMA fiber should be embedded in engineering structure material such as steel, aluminum, etc. The embedding process in these matrix materials should be studied systematically in the future. Keywords Crack control

SMA fiber Actuator Complex stress function

1 Introduction Crack propagation in solid members is an important reason for structure failure. Many researchers are interested in methods of crack control. With the rise in temperature, contraction of prestrained shape memory alloy (SMA) fiber embedding in matrix makes retardation of crack propagation possible. Rogers et al. [1] proposed that embedded prestrained SMA fiber near crack tip may reduce the stress by contraction effect of SMA under increase of temperature. Photoelastic pictures and finite element analysis show that stress intensity factor (SIF) of a specimen embedded with prestrained SMA fiber decreased as temperature increases [2–4]. To overcome separation of SMA fiber from matrix, surface of SMA fiber is treated chemically [2]. Shimamoto et al. [5–8] and Umezaki et al. [9] indicated that stress at the tip of mode-I crack in epoxy matrix with SMA fiber can be reduced by heating SMA fiber. Quality change in matrix near SMA fiber is observed if the temperature is too high. This kind of quality change damages the contraction effect of SMA fiber on crack closure in matrix. Araki et al. [10, 11] performed a micromechanical model on crack closure considering crack bridging fibers and compared their numerical results with experiment. Experiments in these researches give a possible way in practical use to control crack propagation in a specimen. However, with the rise in temperature, separation of SMA fiber from matrix is inevitable. This kind of separation weakens effect of SMA fiber on crack tip. In other words, effect of those applications is limited by the interfacial debonding. Umezaki [12] proposed a type of spiral SMA wire to prevent separation of SMA wire from matrix. In order to avoid the interface de-cohesion or sliding, Gabry et al. [13] used different surface treatments on SMA wires. Pullout tests and scanning electronic microscopy observations [14] indicated that increasing the number of turns of the twisted NiTi wires strengthens bonding strength between fiber and matrix. Zhou et al. [15–17] studied SMA fiber debonding in matrix. Wang et al. [18] proposed a theoretical model for SMA pullout from an elastic matrix. Hu et al. [19] studied interface failure between SMA fiber and matrix by shear lag model. Considering debonding at the interface between SMA wires and a polymer matrix, Wang [20] estimated the minimum volume fraction of SMA wires required to produce stress for the active crack closure. By finite element simulation, Burton et al. [21] indicated that reverse transformation of SMA wires during heating causes a closure force across the crack.

Mode-I Crack Control by SMA Fiber

7

knotted SMA fiber

h crack

a

a

l s

h

photo of a knot

Fig. 1 A knotted prestrained SMA fiber perpendicular to crack surface

To improve effect of SMA fiber on matrix, small knots on SMA fiber are made by authors. Figure 1 shows configuration of a prestrained SMA fiber with knots at each end. With the rise in temperature, the SMA fiber contracts and the two knots on the fiber locking tightly on matrix by recovery stress. This recovery force may reduce the stress intensity factor at the crack tip and make the crack closure. In this process, the fiber cannot be debonded from matrix totally. Therefore, as an actuator in practical use, knotted SMA fiber can be embedded in matrix to control crack propagation. Relation of stress intensity factor with temperature is an important problem in crack control. In this paper, an approximate model on stress intensity factor of mode-I crack closure in matrix is proposed on a specimen with embedded SMA fiber with knots.

2 Relation of Recovery Force on Matrix with Temperature See Fig. 1. Considering a specimen with a mode-I crack in matrix embedded with a prestrained SMA fiber with knots in martensite. SMA fiber is perpendicular to crack surface. Plane strain problem is considered. 2a and 2h denote length of crack and length between the two knots, respectively. l denotes distance from the right crack tip to the fiber. With the rise in temperature, the knotted SMA fiber contracts due to phase transformation from martensite to austenite. The SMA fiber generates a couple of recovery forces P at upper knot Z0 and P at lower knot Z 0 acting on matrix where Z0 ¼ a þ l þ ih;

ð1Þ

8

M. Jin and S. H. Chen

Fig. 2 A couple of recovery forces, P acting on matrix

P y Z0 h x l

h

Z

0

P

Z 0 denotes conjugate of Z0 ; and i denotes imaginary unit. See Fig. 2. Because bonding on interface between fiber and matrix is much weaker than locking between knot and matrix, interfacial shear stress is neglected in this paper. Therefore, the knotted SMA fiber is in simple tension by axial load, P. We have P ¼ srf ;

ð2Þ

where rf and s denote recovery stress and area of the SMA fiber, respectively. In phase transformation, strain of SMA fiber is about several percent which is one order higher than strain of epoxy in elastic range. So we neglect strain of matrix when we consider strain of SMA fiber. Because each knot is locked in the matrix as the fiber contracts, increase of normal strain of SMA fiber embedding in the matrix is approximately zero, i.e. def ¼ 0;

ð3Þ

where ef denotes normal strain of SMA fiber in phase transformation. Based on the Tanaka one-dimensional constitutive law on SMA [22], we have drf ¼ Ef def þ H dT þ X dn;

ð4Þ

where Ef denotes Young’s modulus; H denotes thermoelastic modulus; and X denotes phase transformation modulus. If eL denotes maximum residual strain, we have X ¼ Ef eL in SMA fiber. drf , dT and dn denote increase of normal stress, rise in temperature and increase of martensitic volume fraction of SMA fiber. Martensitic volume fraction, n is a function of stress, rf and temperature, T , i.e., n ¼ n rf ; T : ð5Þ Substituting Eqs. 3 to 5 into 4, we have increase of recovery stress

Mode-I Crack Control by SMA Fiber Fig. 3 Recovery stress, rf versus temperature, T

f

9

£¨ MPa£©

600

400

200

0 40

50

60

70

o

T(C)

drf ¼

on H þ X oT on 1 X or f

dT :

ð6Þ

In phase transformation from martensite to austenite with rise in temperature, function (5) can be approximated by an exponential function [22] with respect to temperature, T , i.e., ð7Þ n ¼ exp aA ðAs T Þ þ bA rf ; aA ln 10 where aA ¼ 2 As Af ; bA ¼ CA ; As and Af are austenite start temperature and austenite finish temperature of SMA fiber, respectively; CA denotes influence coefficient of stress on transition temperature. Substituting Eq. 7 into 6, we have H aA X exp aA ðAs T Þ þ bA rf dT : drf ¼ ð8Þ 1 bA X exp aA ðAs T Þ þ bA rf

Before heating the SMA fiber, stress in theSMA fiber is zero as temperature, T As . The initial value of rf in Eq. 8 is rf T¼As ¼ 0. Generally, we can solve initial value problem (8) numerically by the Euler iteration. However, in Appendix A, we have an analytical solution of initial value problem (8) on martensitic volume fraction, n 8 ln n bA Xðn 1Þ > > þ As ln n aA ðAs T Þ > : rf ¼ bA where n decreases at 1. For a given n, we can get T and rf from Eq. 9. Substituting the value of rf into Eq. 2, we have relation of point load, P with temperature, T : Figure 3 shows curve of recovery stress, rf versus temperature, T .

10

M. Jin and S. H. Chen

Table 1 Material Properties of NiTi Fiber [16, 21] eL As Af Ef 37.4 GPa

0.067

37.7oC

47.2oC

H

CA

9.1 MPa/oC

20.3 MPa/oC

3 Stress Intensity Factor of Mode-I Crack Closure Under a Couple of Point Loads Complex stress function of an elliptic hole in plane strain under a point load is given by [23]. The elliptic hole degenerates into a crack in Fig. 1 as perpendicular axis of elliptic hole tends to zero. Thus we can get complex stress function of the crack under a point load. Based on this complex stress function, we can get stress intensity factor of mode-I crack closure under a couple of point loads P in Fig. 2. The formulation can be seen in Appendix B. Considering Eq. 2, we have ( #) " pﬃﬃﬃ 2 rf 1 1 f a 0 þ ð1 þ m0 ÞIm f0 þ Re ; KI ¼ pﬃﬃﬃ 2Im f0 1 f0 s p ðf0 þ 1Þðf0 1Þ3 ð10Þ where KI is the stress intensity factor of mode-I crack closure, f0 is given by a 1 m where m denotes Poisson’s ratio of matrix; ReðÞ and ImðÞ Z0 ¼ 2 f0 þ f0 ; m0 ¼ 1m denote real component and imaginary component of ðÞ, respectively. Recovery stress, rf can be calculated numerically from Eq. 8 under a temperature, T or analytically from Eq. 9. Substituting recovery stress, rf into Eq. 10, we have the stress intensity factor, KI of mode-I crack closure. Then we have relation of the stress intensity factor, KI of mode-I crack closure with temperature, T .

4 Numerical Results Material properties of SMA fiber are listed in Table l, where Ef denotes Young’s modulus; eL denotes maximum residual strain; As denotes austenite start temperature; Af denotes austenite finish temperature; H denotes thermoelastic modulus; CA denotes influence coefficient of stress on transition temperature. Poisson’s ratio of matrix is m ¼ 0:3. Figure 3 shows curve of recovery stress, rf versus temperature, T . It is shown that recovery stress, rf reaches about 600 MPa as temperature rises to 70 C. Figure 4 shows martensitic volume fraction, n as a function with respect to temperature, T in phase transformation in Figs. 5, 6, 7, 8 and 9. It is shown that martensitic volume fraction, n decreases as the temperature rises from 40 to 70 C:

Mode-I Crack Control by SMA Fiber Fig. 4 Martensitic volume fraction, ξ versus temperature, T

11

1.00

0.95

0.90

0.85

40

50

60

o

70

T ( C)

Fig. 5 The closure stress intensity factor, KI versus temperature, T for different fiber position as h/a = 1.0

a

1/2

K I /s ( Pa ) l/a = -1.0

0

-0.8 -100

-0.6

-200

-0.4

-300 -400 -500 40

50

60

70

T ( oC )

a

1/2

K I /s ( Pa )

l / a = 0.8

0.6 0.4

0

0.2 -100 -200 0.0

-300

-0.2

-400 -500 40

50

T ( oC )

60

70

12 Fig. 6 The closure stress intensity factor, KI versus fiber position, l/a at different temperature as h/a = 1.0

M. Jin and S. H. Chen a

1/2

K I /s ( Pa ) o

0

T = 40 C 45

-100

50 55

-200

60 65

-300

70 -400 -500

l/a -1.5

Fig. 7 The closure stress intensity factor, KI versus fiber position, l/a at different temperature as h/a = 0.1

-1.0

-0.5

0.0

0.5

1.0

1/2

a K I /s ( Pa ) T = 40o C 0 45 -500

50 55

-1000

60 65

-1500 70

l/a -2000 -1.5

Fig. 8 The closure stress intensity factor, KI versus fiber position l/a at different temperature as h/a = 2.0

-1.0

-0.5

0.0

0.5

1.0

-0.5

0.0

0.5

1.0

1/2

a K I /s ( Pa ) 0

T = 40 oC 45

-100

50 55 60

-200

65 70

-300 -1.5

l/a -1.0

As crack length is the same as fiber length, i.e. ha ¼ 1:0, Fig. 5 shows the stress intensity factor of mode-I crack closure as function with respect to temperature for different fiber position. It is shown that stress intensity factor decreases almost

Mode-I Crack Control by SMA Fiber Fig. 9 The closure stress intensity factor, KI versus fiber position l/a at different fiber length

13

1/2

a K I /s ( Pa )

T = 40 oC

0

-40 1.5 1.0

-80

0.5 h /a = 0.1

-120

l/a -1.0

-0.5

0.0

0.5

1.0

linearly with rise in temperature. It is shown that stress intensity factor may take the minimum value at the same temperature between al ¼ 0:2 and 0:4. Figure 6 shows closure stress intensity factor as a function with respect to fiber position at different temperature. At the same temperature, the nearer the fiber locates the crack tip, the little the stress intensity factor is. Effect of crack closure of the fiber behind crack tip is more obvious than that of the fiber in front of crack tip. It is also shown that there is an optimal position for fiber where the stress intensity factor takes the minimum value. For ha ¼ 1:0, this optimal position for effect of crack closure is approximately at al ¼ 0:3 behind the crack tip. Figures 7 and 8 show the stress intensity factor of mode-I crack closure as a function with respect to fiber position at different temperature for ha ¼ 0:1 and 2:0, respectively. Approximately l a ¼ 0:04 and 0:45 are the optimal position for effect of crack closure for h a ¼ 0:1 and 2:0, respectively. Figure 9 shows the closure stress intensity factor as a function with respect to fiber position al for different fiber length ha at temperature 40 C. Near the crack tip, it is shown that, the more short distance of the two knots is, the more obvious the effect of crack closure is. In other words, the nearer the knot locates the crack tip, the more obvious effect of crack closure is.

5 Conclusions Based on the Tanaka one-dimensional constitutive law on SMA, an approximate model on stress intensity factor of mode-I crack closure by prestrained knotted SMA fiber in martensite is proposed. Relation of the stress intensity factor of mode-I crack closure with temperature is given in Eqs. 8 and 9. Numerical results show that the stress intensity factor of mode-I crack closure increases as the prestrained knotted SMA fiber in martensite is heated. Optimal position of the knotted SMA fiber for crack closure is behind the crack tip. As an actuator in

14

M. Jin and S. H. Chen

matrix, prestrained knotted SMA fiber in martensite can be used to control mode-I crack opening. Acknowledgments Authors gratefully acknowledge support from Opening Fund of State Key Laboratory of Nonlinear Mechanics (LNM) of Chinese Academy of Sciences, P. R. China, through grant number LNM201003 and the Science Foundation of Beijing Jiaotong University through grant number PD-225.

Appendix A From derivative of Eq. 7 with respect to temperature, T , we have drf 1 dn ¼ þ aA : dT bA ndT

ðA1Þ

Substituting Eqs. 7 and (A1) into 8, we have 1 bA X dn ¼ ðbA H aA ÞdT : n

ðA2Þ

Indefinite integral of Eq. A2 is ln n bA Xn þ c: ðA3Þ b A H aA where c is a constant. Substituting rf T ¼As ¼ 0 into Eqs. 7 and A3, we have T¼

c¼

bA X þ As : b A H aA

ðA4Þ

Substituting Eq. A4 into A3, we have the first equation in Eq. 9. The second equation in Eq. 9 can be got easily from Eq. 7.

Appendix B Complex stress functions UðfÞ and vðfÞ of an elliptic hole in plane strain under a point load P at Z0 in Fig. 2. are given in Eqs. 4 and 5 in article of [23], respectively. As perpendicular axis of the elliptic hole tends to zero, we have derivatives of UðfÞ and vðfÞ with respect to f 8 2

39 ! > > 1 1 = 2< f þ þ f 0 0 f0 7 dUðfÞ iPa 1 1 f0 0 0 6 1 ¼ þ 1 þ m ð3 m Þ ð Þ þ 5 4

2 2 > 8p > df f f0 f 1 f ; : f0 f0 1 f 1 f0

ðB1Þ

Mode-I Crack Control by SMA Fiber

15

and

39 1 1 = f f þ þ 0 0 f0 dvðfÞ iPa 3m 1 1 f0 5 ; ðB2Þ

þ ð1 þ m0 Þ4 ¼ þ ; 8p :f f0 df f 1 f ðf f0 Þ2 1 f12 f0 8

2

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close